 Nano Express
 Open Access
 Published:
Effective Light Absorption Using the Doublesided Pyramid Gratings for ThinFilm Silicon Solar Cell
Nanoscale Research Lettersvolume 13, Article number: 192 (2018)
Abstract
The design of doublesided pyramid grating structure can be used to enhance broadband light absorption. The front grating can greatly reduce the light reflection, especially in the shortwavelength region, and the rear grating can also achieve that same effect in the longer wavelength region. In the paper, for the doublesided pyramid grating structure, the photon absorption distribution of each part is studied and compared with the bare crystalline silicon. Theoretical results show that, by reasonably adjusting the structure parameters of the doublesided grating, the light reflection of the whole band can be reduced greatly which is beneficial for black silicon formation and the total light absorption is also increased. However, further studies have shown that using the rear grating does not improve the effective light absorption of the crystalline silicon.
Background
With the progress in microfabrication technology, nanometer surface morphology and structure design have become more common and really important [1, 2]. The optimization design of parameters has become more urgent and necessary, especially for the crystalline silicon (CS) thinfilm solar cells [3,4,5,6]. There are some reports on the doublesided grating design applied to CS thinfilm solar cells, and all of them have expressed similar opinions that such a structure can achieve broadband light absorption enhancement which is able to reach the Yablonovitch limit [7,8,9,10]. There is no doubt that the doublesided grating design can improve the overall light trapping capability of CS solar cells. After all, the generation and separation of electronhole pairs occurs inside the CS, and considering each absorbed photon with energy greater than the band gap produces one and only one electronhole pair, so how the photon absorption is distributed among the various parts of the CS solar cell is the focus of this article. In addition, increasing the photon absorption of CS itself to the maximum by adjusting parameters is our aim.
In this paper, the photon absorption distributions of the front pyramid grating (FPG), the rear pyramid grating (RPG), and the doublesided pyramid grating (DSPG) are studied. The total photon absorption A is further divided into three different parts as shown in Fig. 1, the photon absorption of the front surface gratings, the CS part, and the rear surface gratings and labelled as A_{F}, A_{Si}, and A_{R}, respectively. The light reflection R, transmission T, and total absorption A satisfy R + T + A = 1. A_{Si} is not calculated in the same way for different structure models.
Methods
In our theoretical calculations, the net radiation method and effective medium approximation are used together because of the good matching between simulation and experimental results [4, 11]. As shown in Fig. 2, a multilayer medium system of N layers, N_{i} is the complex refractive index of the ith medium and the interfaces are labeled i = 1, …, N − 1, where i is the total number of interfaces. Subscripts a, d and b, c represent the incoming and outgoing electromagnetic radiation, respectively. The relations between the outgoing and incoming energy fluxes (Q) at each interface can be expressed in terms of the reflection at the interface and the transmission passing through the medium. For every interface i, there are four equations,
r_{i,i + 1} and t_{i,i + 1} (r_{i,i + 1} + t_{i,i + 1} = 1) are the reflectivity and transmissivity, respectively, which are determined using Fresnel’s laws at each of the interfaces. The subscripts indicate energy fluxes transferring from layer i to layer i + 1 and vice versa. τ_{i} is the absorption attenuation rate of layer i, defined by
where α_{i} = 4πk_{i}/λ is the absorption coefficient of layer i and d_{i}/cos(φ_{i}) is the distance travelled through the layer of thickness d_{i} with propagation angle φ_{i}. k_{i} is the imaginary part of the complex refractive index N_{i} = n_{i} − ik_{i}. Both the real refractive index n_{i} and the extinction coefficient k_{i} are functions of λ. Assuming the perpendicular incident energy flux Q_{1,a} = 1 and Q_{N,d} = 0, then, for each layer i, the energy absorption coefficient A_{i} = Q_{i,a} − Q_{i,c} + Q_{i,d} − Q_{i,b} can be worked out.
The effective multilayer structure of silicon pyramid is also shown in Fig. 2, and the complex refractive indices of different layers can be solved by the effective medium approximation formula,
where f_{1} and f_{2} are the ratio of volume filling of silicon pyramid gratings and the air, respectively, and f_{1} + f_{2} = 1. N_{Si}, N_{Air}, and N_{Eff} are the complex refractive indices of CS, air, and the interlayer of silicon pyramid gratings, respectively.
Combining the above formulas, the absorbed photon flux of each layer can be calculated by the following formula,
A_{i} is the energy absorption coefficient of each layer; F(λ) is the distribution of solar radiation spectral intensity on the Earth’s surface under AM1.5 spectrum. λ is the wavelength of incident light, h_{0} and c_{0} are the Planck constant and speed of light in vacuum, respectively. The total number of absorbed photon can be expressed as Φ = ∑ Φ_{i}.
Results and Discussion
For the different pyramid grating structures, and for comparison purposes, the related parameters are selected as follows. Firstly, the thickness of CS layer H = 10 μm; the height and bottom diameter of silicon pyramid are set H_{1} = H_{2} = 200 nm and D_{1} = D_{2} = 100 nm, respectively. For FPG, the ratio of period to bottom diameter is set P_{1}/D_{1} = 1, and for RPG, two ratios P_{2}/D_{2} = 1 and P_{2}/D_{2} = 10 are considered. Finally, for DSPG, the different combinations of the above parameters are compared.
The optical performances of different pyramid grating structures under the given parameters are shown in Fig. 3. As can be seen from Fig. 3 (a) and (b), the front surface gratings can greatly reduce the light reflection of the whole band and improve the total light absorption, especially in regions I and II. Meanwhile, in region II, the absorption of infrared light can be improved by the rear surface gratings under proper ratio parameters (P_{2}/D_{2} = 10). Therefore, using them together, for DSPG, adjusting the right parameters not only can they maximize the light absorption to the Yablonovitch limit [7], but also achieve the zero light reflection of the whole band which can make the true black silicon. In addition, the rear surface pyramid gratings can increase transmission of the visible and nearinfrared light seen from Fig. 3 (c), which is beneficial to be used in nearinfrared photodetectors and other fields [9, 10].
For the CS solar cells, greatly enhancing the light absorption especially in the CS body is the ultimate goal. Therefore, it is necessary to study further the distribution of absorbed photons between various parts. For the FPG structure and RPG structure, threedimensional contour maps of photon absorption in each part are shown in Fig. 4 and Fig. 5, respectively.
For the FPG structure, changing the geometric parameters of pyramid arrays, the overall photon absorption distribution compared with the photon absorption distribution of each part is shown in Fig. 4. It can be seen from Fig. 4 (a) that the total absorbed photons increase with the higher height of the pyramid, whereas the larger ratio of period to diameter is not effective for photon absorption. So, it means that the higher height and together with the smaller gap will harvest more highfrequency photons and the same seems true for the FPG absorption shown in Fig. 4 (b). However, if the height of the FPG continues to increase, it reduces the photon absorption of the CS located below as shown in Fig. 4 (c). Obviously, there is an optimal parameter configuration where P_{1}/D_{1} = 1.05, H_{1} = 53 nm. Furthermore, if it is assumed that the photons absorbed by the silicon pyramid are not involved in the conversion of electronhole pairs in the CS, based on these calculations, the suitable ranges of the FPG geometric parameters are also obtained and compared with the bare silicon shown in Fig. 4 (c). In short, the higher the height of FPG, the lower the reflectivity, but this does not mean there is more effective light absorption.
In the same way, for the RPG structure, the photon absorption distributions of the whole and each part are shown in Fig. 5. For the total absorption shown in Fig. 5 (a), compared with the FPG structure, there shows a significant difference in that photon absorption is enhanced with the larger ratio of period to bottom diameter and the lower pyramid height. This means that, on one hand, the larger ratio of P_{2}/D_{2} and smaller H_{2} reduce the lowfrequency photon transmission and the photons turn back, thereby increasing the reflection. But, on the other hand, photons are promoted to be absorbed in the process. Obviously, the parameter configuration which results in the least absorption is P_{2}/D_{2} = 1.01, H_{2} = 168 nm, and the suitable ranges of the RPG geometric parameters are also obtained compared with the bare silicon shown in Fig. 5 (a). However, on the CS part shown in Fig. 5 (b), there is no obvious improvement in the effective light absorption because a large number of photons are reflected. Figure 5 (c) shows that the photons absorbed by the rear surface grating are two orders of magnitude lower than those absorbed by CS, and there is a similar trend which looks like that of the total absorption shown in Fig. 5 (a). Here also, the parameters configuration are P_{2}/D_{2} = 1.03 and H_{2} = 170 nm and almost the same as above.
As seen from the absorption distribution of the FPG and the RPG, the former obviously plays an important role in improving the photon absorption shown in Fig. 4 (c), while the latter implies that photon absorption in the CS part is weakened because of the existence of the rear surface gratings shown in Fig. 5 (b). Combining the findings above, the optical properties of the four sets of different parameters which are representative of the DSPG are studied and shown in Fig. 6.
Due to the weak transmission ability of highfrequency photons shown in Fig. 6 (b), if the ratio of period to bottom diameter is not appropriate (P_{1}/D_{1} = 10 and H_{1} = 10 nm), not only does it not reduce the reflectivity, but it also causes the reflection to increase and the absorption to decrease as shown in Fig. 6. Only suitable parameters (P_{1}/D_{1} = 1.05 and H_{1} = 53 nm) can achieve significant enhancement of light absorption. For the CS, because of its own inability to absorb the lower frequency photons as shown in the region III, the modulation of the front and rear surface gratings only affects the distribution of light between the reflection and transmission. It becomes obvious that the rear gratings are playing a major role in region II and region III, and with the suitable match of the front surface gratings parameters (P_{1}/D_{1} = 1.05, H_{1} = 53 nm, and P_{2}/D_{2} = 1.03, H_{2} = 170 nm), nearly zero reflection of full wave band can be realized. Compared with the FPG of the same parameters, for the total absorption shown in Fig. 6 (c), in region II, the presence of the rear surface gratings with appropriate parameters can actually improve the infrared light absorption (P_{2}/D_{2} = 10, H_{2} = 10 nm), which confirms previous conclusions that the mismatched double grating design can enable significant improvements in device performance [10]. However, for the absorption of the CS part shown in Fig. 6 (d), using the design of rear surface gratings has little effect in improving light absorption of CS. Therefore, in this sense, although the RPG can reflect light and redirect it back toward the photoactive regions of the solar cell [12], it does provide no added benefit for the effective light absorption. Some novel designs to tune absorption spectrum for an optimized integration need to be developed [1, 13].
Conclusions
The design of doublesided pyramid grating structure is adopted to promote the overall light absorption of the silicon solar cell, and it can also realize the zero reflection by adjusting the parameters. However, for the effective light absorption of CS part, it does not increase with the enhancement of the overall light absorption. For the front surface pyramid gratings, the suggested ratio of P_{1}/D_{1} is less than 1.4 and H_{1} is between 10 and 600 nm, and for the rear surface pyramid gratings, there is little effect on the effective light absorption enhancement, so no rear gratings are necessary. Therefore, the innovation and optimized design of the front surface texture is a big trend for further improvement of solar cell efficiency.
Abbreviations
 CS:

Crystalline silicon
 DSPG:

Doublesided pyramid grating
 FPG:

Front pyramid grating
 RPG:

Rear pyramid grating
References
 1.
Leung SF, Zhang Q, Tavakoli MM, He J, Mo X, Fan Z (2016) Progress and design concerns of nanostructured solar energy harvesting devices. Small 12(19):2536–2548
 2.
Green MA, Bremner SP (2016) Energy conversion approaches and materials for highefficiency photovoltaics. Nat Mater 16(1):23–34
 3.
Lin Q, Bo H, Leung Sf, Duan X, Fan Z (2013) Efficient light absorption with integrated nanopillar/nanowell arrays for threedimensional thinfilm photovoltaic applications. ACS Nano 7(3):2725–2732
 4.
Duan Z, Li M, Mwenya T, Fu P, Li Y, Song D (2016) Effective light absorption and its enhancement factor for silicon nanowirebased solar cell. Appl Opt 55(1):117–121
 5.
Duan Z, Li M, Mwenya T, Bai F, Li Y, Song D (2014) Geometric parameter optimization to minimize the lightreflection losses of regular vertical silicon nanorod arrays used for solar cells. Phys Status Solidi A 211:2527–2531
 6.
Shen X, Wang Q, Wangyang P (2016) Broadband antireflection and light trapping in thin film silicon solar cells with hemisphere arrays. IEEE Photon Technol Lett 28(13):1477–1480
 7.
Wang KX, Zongfu Y, Liu V, Yi C, Fan S (2012) Absorption enhancement in ultrathin crystalline silicon solar cells with antireflection and lighttrapping nanocone gratings. Nano Lett 12:1616–1619
 8.
Alshal MA, Allam NK (2016) Broadband absorption enhancement in thin film solar cells using asymmetric doublesided pyramid gratings. J Electron Mater 45(11):1–10
 9.
Eisenlohr J, Tucher N, Hauser H, Graf M, Benick J, Bläsi B, Goldschmidt JC, Hermle M (2016) Efficiency increase of crystalline silicon solar cells with nanoimprinted rear side gratings for enhanced light trapping. Sol Energy Mater Sol Cells 155:288–293
 10.
Hsu WC, Tong JK, Branham MS, Huang Y, Yerci S, Boriskina SV, Chen G (2016) Mismatched front and back gratings for optimum light trapping in ultrathin crystalline silicon solar cells. Opt Commun 377:52–58
 11.
Santbergen R, van Zolingen RJC (2008) The absorption factor of crystalline silicon PV cells: a numerical and experimental study. Sol Energy Mater Sol Cells 92(4):432–444
 12.
Lipovšek B, Krč J, Topič M (2018) Microtextured lightmanagement foils and their optimization for planar organic and perovskite solar cells. IEEE Journal of Photovoltaics 8(3):783–792
 13.
Perl EE, Lin CT, McMahon WE, Friedman DJ, Bowers JE (2014) Ultrabroadband and wideangle hybrid antireflection coatings with nanostructures. IEEE Journal of Photovoltaics 4(3):962–967
Funding
This work was supported partially by the National Hightech R&D Program of China (015AA034601); National Natural Science Foundation of China (51772096, 91333122, 51372082, 51402106, and 11504107); Ph.D. Programs Foundation of Ministry of Education of China (20130036110012); ParEu Scholars Program, Beijing Municipal Science and Technology Project (Z161100002616039); and The Fundamental Research Funds for the Central Universities (2016JQ01, 2015ZZD03, 2015ZD07, 2017ZZD02).
Availability of Data and Materials
Raw data and materials are available on reasonable request.
Author information
Affiliations
Contributions
DZ performed the majority of the theoretical work including the establishment of a theoretical model, data calculation, analysis, and interpretation; under the supervision of LM, TMC is responsible for the revision of the article, especially the language aspect. All authors played key roles in the theoretical design and drafting of the manuscript. Critical revision and approval of the final manuscript was provided by all authors.
Corresponding author
Correspondence to Li Meicheng.
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Received
Accepted
Published
DOI
Keywords
 Geometric Optical Design
 Nanomaterials
 Thin Films
 Solar Energy